 
data_anna2 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'H7.20 Al F3 K0.23 N1.77 O4 S' 
_chemical_formula_weight          221.09 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'N'  'N'   0.0061   0.0033 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Al'  'Al'   0.0645   0.0514 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'S'  'S'   0.1246   0.1234 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'K'  'K'   0.2009   0.2494 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'F'  'F'   0.0171   0.0103 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            ? 
_symmetry_space_group_name_H-M    ? 
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x+1/2, -y+1/2, z+1/2' 
 '-x, y, -z+1/2' 
 'x+1/2, -y+1/2, -z' 
 '-x, -y, -z' 
 'x-1/2, y-1/2, -z-1/2' 
 'x, -y, z-1/2' 
 '-x-1/2, y-1/2, z' 
 
_cell_length_a                    11.289(2) 
_cell_length_b                    8.598(2) 
_cell_length_c                    6.8510(10) 
_cell_angle_alpha                 90.00 
_cell_angle_beta                  90.00 
_cell_angle_gamma                 90.00 
_cell_volume                      665.0(2) 
_cell_formula_units_Z             4 
_cell_measurement_temperature     293(2) 
_cell_measurement_reflns_used     ? 
_cell_measurement_theta_min       ? 
_cell_measurement_theta_max       ? 
 
_exptl_crystal_description        ? 
_exptl_crystal_colour             ? 
_exptl_crystal_size_max           0.12 
_exptl_crystal_size_mid           0.03 
_exptl_crystal_size_min           0.02 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     2.208 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              448 
_exptl_absorpt_coefficient_mu     0.798 
_exptl_absorpt_correction_type    ? 
_exptl_absorpt_correction_T_min   0.9103 
_exptl_absorpt_correction_T_max   0.9842 
_exptl_absorpt_process_details    ? 
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       293(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   ? 
_diffrn_measurement_method        ? 
_diffrn_detector_area_resol_mean  ? 
_diffrn_standards_number          ? 
_diffrn_standards_interval_count  ? 
_diffrn_standards_interval_time   ? 
_diffrn_standards_decay_%         ? 
_diffrn_reflns_number             14472 
_diffrn_reflns_av_R_equivalents   0.0650 
_diffrn_reflns_av_sigmaI/netI     0.0496 
_diffrn_reflns_limit_h_min        -17 
_diffrn_reflns_limit_h_max        18 
_diffrn_reflns_limit_k_min        -10 
_diffrn_reflns_limit_k_max        13 
_diffrn_reflns_limit_l_min        -10 
_diffrn_reflns_limit_l_max        11 
_diffrn_reflns_theta_min          2.98 
_diffrn_reflns_theta_max          35.28 
_reflns_number_total              1478 
_reflns_number_gt                 916 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        ? 
_computing_cell_refinement        ? 
_computing_data_reduction         ? 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     ? 
_computing_publication_material   ? 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0410P)²+0.4900P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     mixed 
_refine_ls_extinction_method      SHELXL 
_refine_ls_extinction_coef        0.006(2) 
_refine_ls_extinction_expression 
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^' 
_refine_ls_number_reflns          1478 
_refine_ls_number_parameters      67 
_refine_ls_number_restraints      4 
_refine_ls_R_factor_all           0.0902 
_refine_ls_R_factor_gt            0.0386 
_refine_ls_wR_factor_ref          0.0977 
_refine_ls_wR_factor_gt           0.0815 
_refine_ls_goodness_of_fit_ref    1.009 
_refine_ls_restrained_S_all       1.011 
_refine_ls_shift/su_max           0.000 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
N N 0.69395(14) 0.32039(17) 0.2072(2) 0.0334(6) Uani 0.845(4) 1 d PD . . 
K K 0.69395(14) 0.32039(17) 0.2072(2) 0.0334(6) Uani 0.155(4) 1 d P . . 
Al Al 0.5000 0.0000 0.0000 0.01355(17) Uani 1 2 d S . . 
S S 0.0000 0.19621(7) 0.2500 0.01591(15) Uani 1 2 d S . . 
O1 O -0.09724(15) 0.10380(17) 0.3239(2) 0.0300(4) Uani 1 1 d . . . 
O2 O -0.04722(14) 0.29892(15) 0.09130(19) 0.0196(3) Uani 1 1 d . . . 
F1 F 0.84925(10) 0.45388(13) 0.47814(17) 0.0223(3) Uani 1 1 d . . . 
F2 F 0.5000 0.07776(17) 0.2500 0.0191(3) Uani 1 2 d S . . 
H1 H 0.670(4) 0.348(5) 0.073(4) 0.080 Uiso 0.85 1 d PD . . 
H2 H 0.764(3) 0.373(4) 0.252(6) 0.080 Uiso 0.85 1 d PD . . 
H3 H 0.700(4) 0.214(3) 0.165(6) 0.080 Uiso 0.85 1 d PD . . 
H4 H 0.643(4) 0.318(5) 0.322(5) 0.080 Uiso 0.85 1 d PD . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
N O1 2.787(2) 8_665 ? 
N F1 2.7992(19) . ? 
N F1 2.8744(19) 2_654 ? 
N O1 2.918(2) 2_554 ? 
N O2 3.034(2) 1_655 ? 
N F2 3.0384(19) . ? 
N F1 3.050(2) 7_565 ? 
N O1 3.109(2) 1_655 ? 
N O2 3.274(2) 2 ? 
N O2 3.556(2) 4 ? 
N H1 0.988(19) . ? 
N H2 0.965(19) . ? 
N H3 0.965(19) . ? 
N H4 0.972(19) . ? 
Al F1 1.7538(12) 6_556 ? 
Al F1 1.7538(12) 2_654 ? 
Al F2 1.8386(6) 5_655 ? 
Al F2 1.8386(6) . ? 
Al O2 1.9142(13) 4 ? 
Al O2 1.9142(13) 8_655 ? 
Al N 3.7945(15) 5_655 ? 
Al K 3.7945(15) 5_655 ? 
Al N 4.0419(17) 4_455 ? 
Al N 4.0419(17) 8_755 ? 
S O1 1.4466(16) . ? 
S O1 1.4466(16) 3 ? 
S O2 1.4988(13) 3 ? 
S O2 1.4988(13) . ? 
S K 3.6280(16) 3_655 ? 
S N 3.6280(16) 3_655 ? 
S N 3.6280(16) 1_455 ? 
S K 3.6280(16) 1_455 ? 
S N 3.8245(15) 2 ? 
S N 3.8245(15) 4_455 ? 
S N 3.9142(17) 8_655 ? 
S N 3.9142(17) 6_556 ? 
O1 K 2.787(2) 8_655 ? 
O1 N 2.787(2) 8_655 ? 
O1 K 2.918(2) 2 ? 
O1 N 2.918(2) 2 ? 
O1 N 3.109(2) 1_455 ? 
O1 K 3.109(2) 1_455 ? 
O1 N 4.098(2) 6_556 ? 
O2 Al 1.9142(13) 4_455 ? 
O2 N 3.034(2) 1_455 ? 
O2 K 3.034(2) 1_455 ? 
O2 N 3.274(2) 2_554 ? 
O2 K 3.274(2) 2_554 ? 
O2 N 3.556(2) 4_455 ? 
O2 N 4.224(2) 3_655 ? 
F1 Al 1.7538(12) 2_655 ? 
F1 N 2.8744(19) 2_655 ? 
F1 K 2.8744(19) 2_655 ? 
F1 N 3.050(2) 7_566 ? 
F1 K 3.050(2) 7_566 ? 
F1 N 3.690(2) 8_765 ? 
F2 Al 1.8386(6) 3_655 ? 
F2 K 3.0384(19) 3_655 ? 
F2 N 3.0384(19) 3_655 ? 
F2 N 4.1133(18) 6_556 ? 
F2 N 4.1133(18) 8_755 ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O1 N F1 72.34(6) 8_665 . ? 
O1 N F1 143.84(7) 8_665 2_654 ? 
F1 N F1 143.58(6) . 2_654 ? 
O1 N O1 85.20(6) 8_665 2_554 ? 
F1 N O1 137.69(7) . 2_554 ? 
F1 N O1 68.18(5) 2_654 2_554 ? 
O1 N O2 120.37(7) 8_665 1_655 ? 
F1 N O2 66.13(5) . 1_655 ? 
F1 N O2 88.31(5) 2_654 1_655 ? 
O1 N O2 97.95(6) 2_554 1_655 ? 
O1 N F2 106.88(7) 8_665 . ? 
F1 N F2 131.98(6) . . ? 
F1 N F2 50.74(4) 2_654 . ? 
O1 N F2 88.31(5) 2_554 . ? 
O2 N F2 132.65(6) 1_655 . ? 
O1 N F1 79.42(6) 8_665 7_565 ? 
F1 N F1 73.76(4) . 7_565 ? 
F1 N F1 109.79(6) 2_654 7_565 ? 
O1 N F1 67.03(5) 2_554 7_565 ? 
O2 N F1 49.49(4) 1_655 7_565 ? 
F2 N F1 154.25(6) . 7_565 ? 
O1 N O1 138.33(7) 8_665 1_655 ? 
F1 N O1 66.43(5) . 1_655 ? 
F1 N O1 77.15(5) 2_654 1_655 ? 
O1 N O1 130.47(7) 2_554 1_655 ? 
O2 N O1 45.61(4) 1_655 1_655 ? 
F2 N O1 96.33(6) . 1_655 ? 
F1 N O1 94.46(6) 7_565 1_655 ? 
O1 N O2 81.10(6) 8_665 2 ? 
F1 N O2 84.98(5) . 2 ? 
F1 N O2 95.50(5) 2_654 2 ? 
O1 N O2 127.16(7) 2_554 2 ? 
O2 N O2 132.74(6) 1_655 2 ? 
F2 N O2 48.91(3) . 2 ? 
F1 N O2 154.65(6) 7_565 2 ? 
O1 N O2 89.38(6) 1_655 2 ? 
O1 N O2 96.73(6) 8_665 4 ? 
F1 N O2 168.25(6) . 4 ? 
F1 N O2 47.11(4) 2_654 4 ? 
O1 N O2 42.30(4) 2_554 4 ? 
O2 N O2 124.70(5) 1_655 4 ? 
F2 N O2 46.03(3) . 4 ? 
F1 N O2 109.13(5) 7_565 4 ? 
O1 N O2 123.75(6) 1_655 4 ? 
O2 N O2 89.11(5) 2 4 ? 
O1 N H1 87(2) 8_665 . ? 
F1 N H1 134(3) . . ? 
F1 N H1 69(2) 2_654 . ? 
O1 N H1 6(3) 2_554 . ? 
O2 N H1 92(3) 1_655 . ? 
F2 N H1 93(3) . . ? 
F1 N H1 62(3) 7_565 . ? 
O1 N H1 126(3) 1_655 . ? 
O2 N H1 133(3) 2 . ? 
O2 N H1 47(3) 4 . ? 
O1 N H2 80(2) 8_665 . ? 
F1 N H2 23(2) . . ? 
F1 N H2 134(2) 2_654 . ? 
O1 N H2 119(2) 2_554 . ? 
O2 N H2 47(2) 1_655 . ? 
F2 N H2 152(2) . . ? 
F1 N H2 53(2) 7_565 . ? 
O1 N H2 65(2) 1_655 . ? 
O2 N H2 108(2) 2 . ? 
O2 N H2 162(2) 4 . ? 
H1 N H2 114(3) . . ? 
O1 N H3 161(3) 8_665 . ? 
F1 N H3 123(3) . . ? 
F1 N H3 21(3) 2_654 . ? 
O1 N H3 88(3) 2_554 . ? 
O2 N H3 78(3) 1_655 . ? 
F2 N H3 55(3) . . ? 
F1 N H3 114(3) 7_565 . ? 
O1 N H3 57(3) 1_655 . ? 
O2 N H3 89(3) 2 . ? 
O2 N H3 67(3) 4 . ? 
H1 N H3 88(3) . . ? 
H2 N H3 119(4) . . ? 
O1 N H4 63(2) 8_665 . ? 
F1 N H4 81(3) . . ? 
F1 N H4 109(2) 2_654 . ? 
O1 N H4 121(3) 2_554 . ? 
O2 N H4 141(3) 1_655 . ? 
F2 N H4 59(3) . . ? 
F1 N H4 140(2) 7_565 . ? 
O1 N H4 103(3) 1_655 . ? 
O2 N H4 18(2) 2 . ? 
O2 N H4 91(3) 4 . ? 
H1 N H4 127(4) . . ? 
H2 N H4 104(3) . . ? 
H3 N H4 105(3) . . ? 
F1 Al F1 180.00(7) 6_556 2_654 ? 
F1 Al F2 89.85(4) 6_556 5_655 ? 
F1 Al F2 90.15(4) 2_654 5_655 ? 
F1 Al F2 90.15(4) 6_556 . ? 
F1 Al F2 89.85(4) 2_654 . ? 
F2 Al F2 180.0 5_655 . ? 
F1 Al O2 87.82(6) 6_556 4 ? 
F1 Al O2 92.18(6) 2_654 4 ? 
F2 Al O2 91.38(6) 5_655 4 ? 
F2 Al O2 88.62(6) . 4 ? 
F1 Al O2 92.18(6) 6_556 8_655 ? 
F1 Al O2 87.82(6) 2_654 8_655 ? 
F2 Al O2 88.62(6) 5_655 8_655 ? 
F2 Al O2 91.38(6) . 8_655 ? 
O2 Al O2 180.00(7) 4 8_655 ? 
F1 Al N 46.20(4) 6_556 5_655 ? 
F1 Al N 133.80(4) 2_654 5_655 ? 
F2 Al N 52.23(4) 5_655 5_655 ? 
F2 Al N 127.77(4) . 5_655 ? 
O2 Al N 111.88(5) 4 5_655 ? 
O2 Al N 68.12(5) 8_655 5_655 ? 
F1 Al K 46.20(4) 6_556 5_655 ? 
F1 Al K 133.80(4) 2_654 5_655 ? 
F2 Al K 52.23(4) 5_655 5_655 ? 
F2 Al K 127.77(4) . 5_655 ? 
O2 Al K 111.88(5) 4 5_655 ? 
O2 Al K 68.12(5) 8_655 5_655 ? 
N Al K 0.00(5) 5_655 5_655 ? 
F1 Al N 133.80(4) 6_556 . ? 
F1 Al N 46.20(4) 2_654 . ? 
F2 Al N 127.77(4) 5_655 . ? 
F2 Al N 52.23(4) . . ? 
O2 Al N 68.12(5) 4 . ? 
O2 Al N 111.88(5) 8_655 . ? 
N Al N 180.00(5) 5_655 . ? 
K Al N 180.00(5) 5_655 . ? 
F1 Al N 44.52(4) 6_556 4_455 ? 
F1 Al N 135.48(4) 2_654 4_455 ? 
F2 Al N 79.15(3) 5_655 4_455 ? 
F2 Al N 100.85(3) . 4_455 ? 
O2 Al N 45.74(5) 4 4_455 ? 
O2 Al N 134.26(5) 8_655 4_455 ? 
N Al N 69.68(2) 5_655 4_455 ? 
K Al N 69.68(2) 5_655 4_455 ? 
N Al N 110.321(19) . 4_455 ? 
F1 Al N 135.48(4) 6_556 8_755 ? 
F1 Al N 44.52(4) 2_654 8_755 ? 
F2 Al N 100.85(3) 5_655 8_755 ? 
F2 Al N 79.15(3) . 8_755 ? 
O2 Al N 134.26(5) 4 8_755 ? 
O2 Al N 45.74(5) 8_655 8_755 ? 
N Al N 110.321(19) 5_655 8_755 ? 
K Al N 110.321(19) 5_655 8_755 ? 
N Al N 69.679(19) . 8_755 ? 
N Al N 180.00(5) 4_455 8_755 ? 
O1 S O1 113.37(14) . 3 ? 
O1 S O2 109.85(9) . 3 ? 
O1 S O2 107.92(9) 3 3 ? 
O1 S O2 107.92(9) . . ? 
O1 S O2 109.85(9) 3 . ? 
O2 S O2 107.79(11) 3 . ? 
O1 S K 148.87(7) . 3_655 ? 
O1 S K 57.81(7) 3 3_655 ? 
O2 S K 55.20(6) 3 3_655 ? 
O2 S K 102.94(6) . 3_655 ? 
O1 S N 148.87(7) . 3_655 ? 
O1 S N 57.81(7) 3 3_655 ? 
O2 S N 55.20(6) 3 3_655 ? 
O2 S N 102.94(6) . 3_655 ? 
K S N 0.00(5) 3_655 3_655 ? 
O1 S N 57.81(7) . 1_455 ? 
O1 S N 148.87(7) 3 1_455 ? 
O2 S N 102.94(6) 3 1_455 ? 
O2 S N 55.20(6) . 1_455 ? 
K S N 145.77(5) 3_655 1_455 ? 
N S N 145.77(5) 3_655 1_455 ? 
O1 S K 57.81(7) . 1_455 ? 
O1 S K 148.87(7) 3 1_455 ? 
O2 S K 102.94(6) 3 1_455 ? 
O2 S K 55.20(6) . 1_455 ? 
K S K 145.77(5) 3_655 1_455 ? 
N S K 145.77(5) 3_655 1_455 ? 
N S K 0.000(15) 1_455 1_455 ? 
O1 S N 42.13(7) . 2 ? 
O1 S N 134.48(7) 3 2 ? 
O2 S N 68.37(6) 3 2 ? 
O2 S N 114.36(6) . 2 ? 
K S N 119.34(2) 3_655 2 ? 
N S N 119.34(2) 3_655 2 ? 
N S N 62.09(2) 1_455 2 ? 
K S N 62.09(2) 1_455 2 ? 
O1 S N 134.48(7) . 4_455 ? 
O1 S N 42.13(7) 3 4_455 ? 
O2 S N 114.36(6) 3 4_455 ? 
O2 S N 68.37(6) . 4_455 ? 
K S N 62.09(2) 3_655 4_455 ? 
N S N 62.09(2) 3_655 4_455 ? 
N S N 119.34(2) 1_455 4_455 ? 
K S N 119.34(2) 1_455 4_455 ? 
N S N 175.72(5) 2 4_455 ? 
O1 S N 31.61(7) . 8_655 ? 
O1 S N 86.84(7) 3 8_655 ? 
O2 S N 137.71(6) 3 8_655 ? 
O2 S N 103.48(6) . 8_655 ? 
K S N 141.42(5) 3_655 8_655 ? 
N S N 141.42(5) 3_655 8_655 ? 
N S N 72.79(2) 1_455 8_655 ? 
K S N 72.79(2) 1_455 8_655 ? 
N S N 73.16(3) 2 8_655 ? 
N S N 103.19(3) 4_455 8_655 ? 
O1 S N 86.84(7) . 6_556 ? 
O1 S N 31.61(7) 3 6_556 ? 
O2 S N 103.48(6) 3 6_556 ? 
O2 S N 137.71(6) . 6_556 ? 
K S N 72.79(2) 3_655 6_556 ? 
N S N 72.79(2) 3_655 6_556 ? 
N S N 141.42(5) 1_455 6_556 ? 
K S N 141.42(5) 1_455 6_556 ? 
N S N 103.19(3) 2 6_556 ? 
N S N 73.16(3) 4_455 6_556 ? 
N S N 68.72(5) 8_655 6_556 ? 
S O1 K 132.61(10) . 8_655 ? 
S O1 N 132.61(10) . 8_655 ? 
K O1 N 0.00(6) 8_655 8_655 ? 
S O1 K 118.45(9) . 2 ? 
K O1 K 107.87(7) 8_655 2 ? 
N O1 K 107.87(7) 8_655 2 ? 
S O1 N 118.45(9) . 2 ? 
K O1 N 107.87(7) 8_655 2 ? 
N O1 N 107.87(7) 8_655 2 ? 
K O1 N 0.00(6) 2 2 ? 
S O1 N 99.00(8) . 1_455 ? 
K O1 N 98.80(6) 8_655 1_455 ? 
N O1 N 98.80(6) 8_655 1_455 ? 
K O1 N 79.27(5) 2 1_455 ? 
N O1 N 79.27(5) 2 1_455 ? 
S O1 K 99.00(8) . 1_455 ? 
K O1 K 98.80(6) 8_655 1_455 ? 
N O1 K 98.80(6) 8_655 1_455 ? 
K O1 K 79.27(5) 2 1_455 ? 
N O1 K 79.27(5) 2 1_455 ? 
N O1 K 0.00(4) 1_455 1_455 ? 
S O1 N 72.52(7) . 6_556 ? 
K O1 N 77.26(6) 8_655 6_556 ? 
N O1 N 77.26(6) 8_655 6_556 ? 
K O1 N 118.68(6) 2 6_556 ? 
N O1 N 118.68(6) 2 6_556 ? 
N O1 N 162.03(5) 1_455 6_556 ? 
K O1 N 162.03(5) 1_455 6_556 ? 
S O2 Al 132.08(9) . 4_455 ? 
S O2 N 100.86(7) . 1_455 ? 
Al O2 N 107.39(6) 4_455 1_455 ? 
S O2 K 100.86(7) . 1_455 ? 
Al O2 K 107.39(6) 4_455 1_455 ? 
N O2 K 0.000(16) 1_455 1_455 ? 
S O2 N 125.33(7) . 2_554 ? 
Al O2 N 99.28(5) 4_455 2_554 ? 
N O2 N 75.06(4) 1_455 2_554 ? 
K O2 N 75.06(4) 1_455 2_554 ? 
S O2 K 125.33(7) . 2_554 ? 
Al O2 K 99.28(5) 4_455 2_554 ? 
N O2 K 75.06(4) 1_455 2_554 ? 
K O2 K 75.06(4) 1_455 2_554 ? 
N O2 K 0.00(6) 2_554 2_554 ? 
S O2 N 88.56(7) . 4_455 ? 
Al O2 N 81.92(5) 4_455 4_455 ? 
N O2 N 154.89(5) 1_455 4_455 ? 
K O2 N 154.89(5) 1_455 4_455 ? 
N O2 N 80.49(5) 2_554 4_455 ? 
K O2 N 80.49(5) 2_554 4_455 ? 
S O2 N 56.83(5) . 3_655 ? 
Al O2 N 78.72(5) 4_455 3_655 ? 
N O2 N 145.20(4) 1_455 3_655 ? 
K O2 N 145.20(4) 1_455 3_655 ? 
N O2 N 138.93(5) 2_554 3_655 ? 
K O2 N 138.93(5) 2_554 3_655 ? 
N O2 N 58.52(3) 4_455 3_655 ? 
Al F1 N 139.21(7) 2_655 . ? 
Al F1 N 107.67(6) 2_655 2_655 ? 
N F1 N 85.38(4) . 2_655 ? 
Al F1 K 107.67(6) 2_655 2_655 ? 
N F1 K 85.38(4) . 2_655 ? 
N F1 K 0.00(7) 2_655 2_655 ? 
Al F1 N 111.71(6) 2_655 7_566 ? 
N F1 N 104.01(6) . 7_566 ? 
N F1 N 98.25(5) 2_655 7_566 ? 
K F1 N 98.25(5) 2_655 7_566 ? 
Al F1 K 111.71(6) 2_655 7_566 ? 
N F1 K 104.01(6) . 7_566 ? 
N F1 K 98.25(5) 2_655 7_566 ? 
K F1 K 98.25(5) 2_655 7_566 ? 
N F1 K 0.00(5) 7_566 7_566 ? 
Al F1 N 88.75(5) 2_655 8_765 ? 
N F1 N 86.21(5) . 8_765 ? 
N F1 N 162.35(7) 2_655 8_765 ? 
K F1 N 162.35(7) 2_655 8_765 ? 
N F1 N 68.86(3) 7_566 8_765 ? 
K F1 N 68.86(3) 7_566 8_765 ? 
Al F2 Al 137.36(8) . 3_655 ? 
Al F2 N 99.20(4) . . ? 
Al F2 N 109.85(4) 3_655 . ? 
Al F2 K 109.85(4) . 3_655 ? 
Al F2 K 99.20(4) 3_655 3_655 ? 
N F2 K 93.28(7) . 3_655 ? 
Al F2 N 109.85(4) . 3_655 ? 
Al F2 N 99.20(4) 3_655 3_655 ? 
N F2 N 93.28(7) . 3_655 ? 
K F2 N 0.00(4) 3_655 3_655 ? 
Al F2 N 82.57(4) . 6_556 ? 
Al F2 N 74.81(3) 3_655 6_556 ? 
N F2 N 168.97(6) . 6_556 ? 
K F2 N 75.949(19) 3_655 6_556 ? 
N F2 N 75.949(19) 3_655 6_556 ? 
Al F2 N 74.81(3) . 8_755 ? 
Al F2 N 82.57(4) 3_655 8_755 ? 
N F2 N 75.949(19) . 8_755 ? 
K F2 N 168.97(6) 3_655 8_755 ? 
N F2 N 168.97(6) 3_655 8_755 ? 
N F2 N 114.91(6) 6_556 8_755 ? 
 
_diffrn_measured_fraction_theta_max    0.989 
_diffrn_reflns_theta_full              35.28 
_diffrn_measured_fraction_theta_full   0.989 
_refine_diff_density_max    0.376 
_refine_diff_density_min   -0.628 
_refine_diff_density_rms    0.103 
